| ||Format||Pages||Price|| |
|5||$48.00||  ADD TO CART|
|Hardcopy (shipping and handling)||5||$48.00||  ADD TO CART|
|Standard + Redline PDF Bundle||10||$58.00||  ADD TO CART|
This practice describes the general ultrasonic examination procedures for the detection of discontinuities in the weld and adjacent heat affected zones of welded pipe and tubing by scanning with relative motion between the search unit and pipe or tube. When contact or unfocused immersion search units are employed, this practice is intended for tubular products having specified outside diameters and wall thicknesses. And when properly focused immersion search units are employed, this practice may also be applied to material of smaller diameter and thinner wall. This practice does not establish acceptance criteria for this procedure. A pulsed ultrasonic angle beam shall be propagated in the wall of the pipe or tube by either the surface contact or immersion method. The weld line shall then be examined from both sides to ensure detection of imperfections with a shape or orientation that produces a preferential direction of reflection.
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
Significance and Use
5.1 The purpose of this practice is to outline a procedure for detecting weld discontinuities such as lack of fusion, pin holes, lack of penetration, longitudinal cracks, porosity and inclusions by the ultrasonic pulse-reflection method.
1.1 This practice describes general ultrasonic testing procedures for the detection of discontinuities in the weld and adjacent heat affected zones of welded pipe and tubing by scanning with relative motion between the search unit and pipe or tube. When contact or unfocused immersion search units are employed, this practice is intended for tubular products having specified outside diameters ≥2 in. (≥50 mm) and specified wall thicknesses of 1/8 to 11/16 in. (3 to 27 mm). When properly focused immersion search units are employed, this practice may also be applied to material of smaller diameter and thinner wall.
Note 1: When contact or unfocused immersion search units are used, precautions should be exercised when examining pipes or tubes near the lower specified limits. Certain combinations of search unit size, frequency, thin–wall thicknesses, and small diameters could cause generation of unwanted sound waves that may produce erroneous examination results.
1.2 All surfaces of material to be examined in accordance with this practice shall be clean from scale, dirt, burrs, slag, spatter or other conditions that would interfere with the examination results. The configuration of the weld must be such that interfering signals are not generated by reflections from it. Treatment of the inner surface and outer surface weld beads such as trimming (“scarfing”) or rolling is often required to remove protuberances that could result in spurious reflections.
1.3 This practice does not establish acceptance criteria, they must be specified by the using parties.
1.4 The values stated in inch-pound units are to be regarded as the standard. The SI equivalents are in parentheses and may be approximate.
1.5 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
E543 Specification for Agencies Performing Nondestructive Testing
E1316 Terminology for Nondestructive Examinations
ASNT DocumentsANSI/ASNT CP-189 Standard for Qualification and Certification of Nondesctructive Testing Personnel Recommended Practice SNT-TC-1A Personnel Qualification and Certification in Nondestructive Testing
ISO StandardISO 9712 Non-destructive Testing--Qualification and Certification of NDT Personnel
ICS Number Code 23.040.01 (Pipeline components in general. Pipelines)
UNSPSC Code 31311500(Welded or brazed pipe assemblies)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM E273-15, Standard Practice for Ultrasonic Testing of the Weld Zone of Welded Pipe and Tubing, ASTM International, West Conshohocken, PA, 2015, www.astm.orgBack to Top